Physica C 205 ( 1993 ) 307-310 North-Holland
Effect of pressure on the critical current density of YBa2Cu307_~ thin films Q. Xiong, Y.Y. Xue, Y.Y. Sun, P.H. Hor and C.W. Chu Department of Physics and Texas Centerfor Superconductivity, Universityof Houston, Houston, TX 77204-5932, USA
M.F. Davis and J.C. Wolfe Department of Electrical Engineering and Texas Centerfor Superconductivity, Universityof Houston, Houston, TX 77204-5932, USA
S.C. Deshmukh and D.J. Economou Department of Chemical Engineering and Texas Centerfor Superconductivity, Universityof Houston, Houston, TX 77204-5932, USA
Received 13 November 1992
We have investigated the effect of pressure on the critical current density (Jc) at 77 K in YBa2Cu3OT_a thin films with an ambient Jc varying from 104 to 4 × 106 A/cm 2. The same linear enhancement of the relative Jc up to ~ 24 percent at 16 kbar was observed for all samples. The observation can be explained in terms of the internal strain existing in the Y 1: 2: 3 thin films.
Over the last four years, considerable effort has been focused on understanding a n d i m p r o v i n g the critical current density (J~) in YBa2Cu307_ ~ ( Y 1 : 2 : 3) thin films. One outstanding problem is the much greater pinning strength in thin film than in bulk samples. Regardless o f the various synthesis techniques, the J~s o f good thin films seem to converge at 6X 106 A / c m 2 at 77 K, while the Jcs o f good bulk samples seem to be between 104 and 105 A / c m 2. It was d e m o n s t r a t e d [ 1 ] that, while the intragrain J~ o f thin films can be as high as 106 A / c m 2, grain misorientations will reduce the intergrain Jc to l05 A / cm 2 or less. However, single crystals o f Y 1 : 2 : 3, which are supposed to be weak-link free, display a Jc which is orders o f magnitude lower than that o f thin films. This implies that there are stronger pinning centers in thin films. Consequently, much T E M work has been devoted to the search for defects which are unique to thin films. The efforts led to some new discoveries in the microstructure o f thin films . However, such unique defects might not be dense enough to explain a high J~ in epitaxial films [2,3]. In another m o d e l [ 3 ], an extremely high defect-den-
sity was proposed as the m a i n reason for the high Jc in thin films. However, there is no direct T E M evidence for it yet. This puzzle p r o m p t e d us to study the relationship between pinning and strain. Generally, epitaxial thin films are characterized by large inhomogeneous microstrains which, in Y 1 : 2 : 3, could be created by lattice misfit, differences in thermal expansion, and the o r t h o r h o m b i c - t e t r a g o n a l phase transition. Such large internal strain has been observed by X-ray diffraction. Since the internal strain can enhance pinning in the conventional low transition t e m p e r a t u r e Tc superconductors , it is natural to expect a similar effect for Y 1 : 2 : 3. To test this conjecture, the Jcs and Tcs o f Y 1 : 2 : 3 thin films with an a m b i e n t Jc ranging from 104 to 4 × 106 A / c m 2 at 77 K have been measured in a hydrostatic pressure b o m b up to 16 kbar. The J¢ was observed to increase universally with pressure by 24 percent. This suggests that there is a close relationship between the stair and the pinning. The Y 1 : 2 : 3 thin films examined in this study were prepared on SrTiO3 or LaA103 substrates by the laser ablation technique . S t a n d a r d X-ray rocking-
0921-4534/93/$06.00 © 1993 Elsevier Science Publishers B.V. All rights reserved.
Q. Xiong et al. /Effect o f pressure on J~
curve, pole-figure, and peak-profile analysis techniques were employed to obtain microstructural and local strain information on these thin films. A fourprobe method was used to determined J¢ and T¢. For these measurements, 10/~m × 1 mm thin film strips were patterned by the dry-etching technique . Electrical Pt-leads were attached to the strips with In-contacts with a typical contact resistance of ~ 1 fL A 1 ~tV/cm standard was used to measure the Jc. The hydrostatic pressure was generated by the clamp technique , using the Fluorinert (3M Industrial Chemical Co.) as the pressure medium. The pressure was determined by a superconducting Pbmanometer. By varying the deposition conditions, two types of c-oriented films of thickness ~ 2000 A were obtained: type A was epitaxial, single-crystal-like and type B was polycrystalline. Type A films displayed an average mosaic spread of the c-axis A0< 0.3 ° and an average alignment spread of the a, b-axis A0< 1 °. Type B films exhibited a much larger spread of < 1 °. These films had a T¢ between 85 and 91 K and a transition width between ~ 1 and 2 K. Under pressure, the Tc changes negligibly for both types of thin films, with the onset Tc showing a slight increase but the zero-resistivity point showing a small decrease as shown in fig. 1. At 16 kbar, the mid-transition point was hardly shifted, i.e. <0.2 K. Such a pressure effect is small compared to that for bulk Y1:2:3. The pressure coefficient is ~0.04 K/kbar [ 7 ] for bulk Y 1 : 2: 3 with T~= 92 K and increases for samples with lower To. The small effect observed here
may be associated with the complication arising from the nonhydrostaticity of pressure due to the anisotropic nature of the thin-film/substrate sample-system or arising from the large internal strain in the sample-system. On the other hand, the J¢ at 77 K increases clearly with pressure for all samples, as shown in fig. 2. The Jc-enhancement normalized to the ambient Jc was found to be linear for all thin films investigated, as displayed in fig. 3. At 16 kbar, a universal 24 percent Jc-increase was detected. The temperature variation, as monitored by a thermocouple attached to the sample throughout the Jcmeasurements, was less than 0.1 K. 10 ~_..8
~r~ 2 o -1 0.0
J(lo%/om 2) Fig. 2. E - J curves for a typical Y 1 : 2 : 3 thin film (Jc~ 1 × 104 A / cm 2 at 77 K) under various pressures. ( • ) p = 0, ( • ) p = 2.84 kbar, ( * ) p = 8.55 khar, ( • ) p = 15.14 kbar, ( O ) p = 0 (release
12 4 89.0 1.20 88.4
["~8 7.2 •
1.04 86.6 1.00 86.0
P(kbar) Fig. I. T¢ vs. P for a typical Y 1:2:3 thin film. ( O ) Tc~on, ( • )
Tc,,id, ( I ) Tc.....
P(kbar) Fig. 3. The normalized Jc/Jco vs. P for several films. Type I film with ( O ) J¢o = 1.6X 106 and ( * ) J~o=4.1 × 104 A/cm2; type II film with (/x) J¢o=4.8 × 104 and ( I ) Jco= 7.9× 105 A / c m 2.
Q. Xionget al. /Effect ofpressure on Jc It is known that the Jc of a sample at a fixed temperature T increases as Tc increases, or as the reduced temperature t = T! T~ decreases. We have measured the J¢ at different temperatures near 77 K and found that the average temperature coefficient of Jc, ( 1/J~) (dJc/dt) is ~ 0.13. As mentioned above, the pressure-induced T~-increase is less than 0.2 K at 16 kbar. The accompanying J¢-increase is therefore not more than ~ 3 percent, too small to account for the observed J~-enhancement. It has been demonstrated that the J~ of high temperature superconductors is seriously limited by weak links which can be microcracks, second-phase impurities, or large-angle grain boundaries. The application of pressure certainly can close the microcracks or reduce the thickness of the second-phase layers between superconducting grains and increase Jc which has been observed in ceramic samples [ 8 ]. However, for a thin film sample, the pressure-induced strain or the change of the above physical lengths is dictated predominantly by the mechanical stiffness of the substrate, such as SrTiO3 or LaAIO3. At our maximum pressure of 16 kbar, the maximum strain generated cannot be greater than 0.2 percent and is expected to be uniform throughout the entire sample which, again, is too small to affect the weak links by the observed 24 percent, not to mention the unlikelihood of the large effect of microcracks in thinfilm samples with Jc> 10 6 A / c m 2. The effect of misorientation of grains on J¢ has been previously studied [ 1 ]. It was shown that the measured intergrain J¢=J¢of(O), where Jco is the intragrain critical current density and f(O) is a universal decreasing function of the misalignment angle 0 between the grains. The wide spread of J¢ in the thin film samples can be caused by the differences in J¢o and/or f(O), which arise from the different deposition conditions used. Since the pressure effect on the observed Jc is reversible, it is extremely unlikely that such an effect can occur through the orientation of grains, or in other words, through change in f(O). Therefore, our observation suggests that pressure enhances J¢ through a modification in J¢o. It has been proposed  that pinning can be enhanced by a strain field associated with defects. The pinning potential can result from the change in volumes or elastic constants between the superconducting and the normal states. The former depends
on strain (~) linearly, whereas the latter does quadratically. The pinning forces (Fp) in a one-dimensional model are then dE/dx and d(E2)/dx, respectively. In both cases, the flux pinning is proportional to the strain gradient over a length-scale comparable to the coherence length. Externally applied hydrostatic pressure will produce an additional strain (E~). For an anisotropic thin-film/substrate sample-system, such as the one studied here, one can still reasonably assume that the strain induced by the external pressure is uniform along the a, b-plane. E1 is estimated to be __<0.2percent for Y 1 : 2 : 3 thin films at 16 kbar. A uniform el will not affect the linear part of Fp due to the volume change between the superconducting and normal states. However, the quadratical term for Fp becomes d(el + e ) 2 / d x = 2 e l (de/ dx) + de2/dx~2e~ (de/dx), +Fo where Fo is the pinning force in the absence of external pressure. The linear pressure-dependence of J¢ observed in Y1 : 2 : 3 thin films can therefore be understood in terms of the enhanced pinning force induced by pressure associated with the elastic-constant change between the superconducting and normal states. The lattice mismatch and the difference between the thermal expansion coefficients of Y1 : 2:3 and the substrate, the tetragonal-orthorhombic transition, intergrowth, and anisotropy in Y 1 : 2: 3 can be causes for e. However, we would like to point out that the similarity of the observed J¢-enhancements by pressure in various Y 1 : 2 : 3 thin films might imply both a nearly universal pressure effect of the intragrain-pinning (//co) and that the different f(O) (which will not change under pressure) is the main cause of different Jcs in various thin films. Further verification and a detailed explanation are needed. In conclusion, we have observed a linear Jc-enhancement by pressure in various Y 1 : 2 : 3 thin films with Jc ranging from 104 to 4 × 106 A / c m 2. At 16 kbar, a ~ 24 percent J~ increase resulted. The observation can be understood in terms of the increase in pinning associated with the quadratic strain-dependence of the pinning potential proposed . However, further experiments are needed to unravel the implications of the similarity of the J¢-enhancement by pressure.
Q. Xiong et al. /Effect o f pressure on Jc
Acknowledgements T h e a u t h o r s w o u l d like to t h a n k S. B u d ' k o , Y.Q. W a n g a n d Y.K. T a o for helpful discussions. T h i s w o r k is s u p p o r t e d in part by N S F G r a n t No. D M R 91-22043, D A R P A G r a n t No. M D A 972-88-G-002, the State o f Texas, N A S A G r a n t No. N A G W - 9 7 7 , Texas C e n t e r for S u p e r c o n d u c t i v i t y at the U n i v e r sity o f H o u s t o n , a n d the T. L. L. T e m p l e F o u n d a t i o n .
References [ 1 ] D. Dimos, P. Chaudhari, J. Mannhart and F.K. LeGoues, Phys. Rev. Lett. 61 (1988) 219; D. Dimos, P. Chaudhari and J. Mannhart, Phys. Rev. B 41 (1990) 4038.
[2 ] See, for example, G. Gerber, D. Anselmetti, J.G. Bednorz, J. Mannhart and D.G. Schlorn, Nature (London) 350 ( 1991 ) 279. [ 3 ] T.L. Hylton and M.R. Beasley, Phys. Rev. B 41 (1990) 11669. [ 4 ] See, for example, A.M. Campbell and J.E. Everetts, Adv. Phys. 21 (1972) 199.  M.F. Davis, J. Wosik, K. Forster, S.C.Deshmukh, H.R. Rampersad, S. Shah, P. Siemsen, J.C. Wolfe and D.J. Economou, J. Appl. Phys. 69 ( 1991 ) 7182.  C.W. Chu, T.F. Smith and W.E. Gardner, Phys. Rev. Lett. 20 (1968) 198.  Z.J. Huang, P.H. Hot, R.L. Meng, Y.Q. Wang, L. Gao, J. Bechtold, Y.Y. Sun and C.W. Chu, APS Bull. 33 ( 1988 ) 389. [ 8 ] Recently, there have been reports of a large pressure effect on ceramic oxide superconductors, which might be the result of weak-link healing; see, for example, V. Svistunov et al. Mod. Phys. Lett. 4 (1990) 645.